Abstract
Rareearth nickelates form an intriguing series of correlated perovskite oxides. Apart from LaNiO_{3}, they exhibit on cooling a sharp metalinsulator electronic phase transition, a concurrent structural phase transition, and a magnetic phase transition toward an unusual antiferromagnetic spin order. Appealing for various applications, full exploitation of these compounds is still hampered by the lack of global understanding of the interplay between their electronic, structural, and magnetic properties. Here we show from firstprinciples calculations that the metalinsulator transition of nickelates arises from the softening of an oxygenbreathing distortion, structurally triggered by oxygenoctahedra rotation motions. The origin of such a rare triggered mechanism is traced back in their electronic and magnetic properties, providing a united picture. We further develop a Landau model accounting for the metalinsulator transition evolution in terms of the rareearth cations and rationalizing how to tune this transition by acting on oxygen rotation motions.
Introduction
First synthesized in 1971^{1}, rareearth nickelates (RNiO_{3}, with R = rare earth) are appealing for various applications^{2, 3}, and the possibility to tune their properties in epitaxial films and heterostructures^{4} has recently fueled an even larger interest^{5,6,7}. RNiO_{3} compounds belong to the family of perovskite oxides with a reference \(Pm\bar 3m\) cubic structure (Fig. 1a), nevertheless not directly observed. Apart for LaNiO_{3}, which always keeps a metallic \(R\bar 3c\) phase and will not be further discussed here, all RNiO_{3} adopt at reasonably high temperature a metallic Pbnm orthorhombic phase^{8}. This phase, rather ubiquitous^{9} amongst perovskites with small Goldschmidt tolerance factor^{8}, t, corresponds to a distortion of the cubic structure arising from the appearance of combined antiphase rotations of the oxygen octahedra along the x and y directions, R _{ xy } (Fig. 1b), with the same amplitude Q _{R} and inphase rotations of the oxygen octahedra along z, M _{ z } (Fig. 1c), with amplitude Q _{M}.
In this phase, all Ni atoms are equivalent and formally in a JahnTeller active d ^{7} (likely \(t_{{\mathrm{2g}}}^6e_{\mathrm{g}}^1\) low spin) configuration. Surprisingly, although compatible with the Pbnm symmetry, cooperative JahnTeller distortions do not appear. Instead, at a temperature T _{MI}, which strongly evolves with the R cation (i.e., with t)^{10}, RNiO_{3} compounds exhibit an electronic metalinsulator transition (MIT), which was shown to be concurrent with a structural transition from Pbnm to monoclinic P2_{1}/n symmetry^{11}. This symmetry lowering is accompanied with the appearance of a breathing distortion of the oxygen octahedra, B _{OC} (Fig. 1d), which alternatively expand and contract with amplitude Q _{B}, according to a rocksalt pattern. This gives rise to two types of Ni sites with long and short Ni–O bonds, respectively.
At low temperature (100–200 K), RNiO_{3} compounds finally show a magnetic phase transition toward an unusual E′type antiferromagnetic (AFM) spin order identified by a Bragg vector q = (1/4, 1/4, 1/4) in pseudocubic notation^{11,12,13}. For large cations (R = Nd and Pr), the Néel temperature T _{N} = T _{MI} and the system goes directly from paramagnetic metal (PMM) to AFM insulator (AFMI). For smaller R cations, T _{N} is much lower than T _{MI}; the two phase transitions are decoupled and the system goes through an intermediate paramagnetic insulating phase (PMI).
The origin of the MIT has been widely debated in the literature^{14,15,16,17,18,19}. It was sometimes interpreted as a charge disproportionation at Ni sites^{20}: 2(d ^{7}) → d ^{8} + d ^{6}. However, the importance of Ni 3dO 2p hybridization—i.e., transfer of electrons from O to Ni and formation of oxygen holes \(\left( {\underline L } \right)\) keeping Ni in a d ^{8} configuration (i.e., \(d^{8  n} \approx d^8\underline L ^n\))—was evoked early on^{15}. Nowadays, the MIT is usually viewed as a charge ordering of the type \(2\left( {d^8\underline L ^1} \right) \to \left( {d^8} \right) + \left( {d^8\underline L ^2} \right)\) ^{17, 21, 22}. In this scenario, B _{OC} appears important to stabilize the charge ordering and open the gap. As suggested in ref. ^{23} and confirmed from statistical correlation techniques^{24}, R _{ xy } and M _{ z } are also expected to play an active role. However, a complete picture linking electronic, structural and magnetic properties is yet to emerge.
Unlike recent theoretical studies, which were focusing specifically on the electronic properties^{17,18,19, 21}, we investigate here selfconsistently the electronic and structural degrees of freedom of RNiO_{3} compounds from density functional theory calculations (DFT, see Methods). Specific care was given to the validation of our approach, which turns out to provide an unprecedented agreement with experimental data. Focusing on YNiO_{3}, we show (Supplementary Notes 1–4) that not only the atomic structure but also the AFME′ ground state, the estimated T _{N} and the electronic bandgap of the insulating phase are very accurately reproduced, making therefore our approach a method of choice to shed light on the interlink between these different features.
Results
Energetics of individual lattice distortions
We start from the reference \(Pm\bar 3m\) cubic structure. Inspection of the phonon dispersion curves (Supplementary Note 5) reveals dominant structural instabilities at R (ω _{R} = 310i cm^{−1}) and M (ω _{M} = 278i cm^{−1}) points of the Brillouin zone (BZ), which are associated, respectively, to the R _{ xy } and M _{ z } distortions responsible for the Pbnm phase. These imaginary frequencies ω _{i} are linked to a negative energy curvature α _{i} at the origin \(\left( {\alpha _{\mathrm{i}} \propto \omega _{\mathrm{i}}^2 < 0} \right)\) and to a typical doublewell (DW) shape of the energy when freezing R _{ xy } and M _{ z } distortions of increasing amplitude within the cubic structure, as illustrated in Fig. 1. These wells are nearly independent of the spin order but strongly evolve with the R cation: they become shallower when R size increases, consistently with a reduction of the related distortion amplitudes in the Pbnm phase.
In contrast, the B _{OC} motion, corresponding to another phonon at R, is stable and extremely stiff (in fact the stiffest mode with ω _{B} = 700 cm^{−1}), in line with the singlewell (SW) shape illustrated in Fig. 1. Decreasing R cation size tends to stabilize slightly further B _{OC}, in apparent contradiction with the observed increase of T _{MI}. As illustrated for YNiO_{3}, switching from ferromagnetic (FM) to AFME′ spin order reduces slightly the curvature but does not reverse it; instead it shifts the SW to lower energy^{13}, yielding a finite Q _{B} at the minimum. Although B _{OC} tends to make the system insulating, this amplitude (25% of ground state’s value) is however not large enough to open a gap (more than 75% would be required). This shows that B _{OC} and the magnetic order alone cannot explain the MIT by themselves.
Mode coupling and triggered mechanism
Our central result is presented in Fig. 2 where we report in panel a the evolution of the B _{OC} energy well of YNiO_{3} at various fixed amplitudes of oxygen rotation motions. It highlights that although initially stable (SW), B _{OC} is progressively destabilized (DW) by the appearance of R _{ xy } and M _{ z }. As illustrated in panel b, α _{B} is renormalized into \(\tilde \alpha _{\mathrm{B}}\), which evolves linearly with \(Q_{\mathrm{R}}^2\) and \(Q_{\mathrm{M}}^2\). The slope associated to Q _{R} is twice as large as that related to Q _{M}, attesting that each of the three individual rotations similarly affects B _{OC}. This behavior arises from the presence in the energy expansion of cooperative (λ < 0) biquadratic coupling terms between B _{OC} and oxygen rotations (\(E \approx \lambda _{{\mathrm{Bi}}}Q_{\mathrm{B}}^{\mathrm{2}}Q_{\mathrm{i}}^{\mathrm{2}}\), i = M,R), which, being the lowestorder couplings allowed by symmetry, should give rise to the appearance of B _{OC} through a triggered phase transition according to Holakovsky^{25}. The same behavior is observed independently of the magnetic order (Supplementary Note 8). From now we focus on representative FM results while coming back to the role of magnetism later.
Landau model and phase diagram
To further assess the relevance of such a triggered mechanism in nickelates, we built a Landau model, including R _{ xy }, M _{ z }, and B _{OC} degrees of freedom^{24}, restricting ourselves to lowest coupling terms and assuming temperature dependence of the oxygen rotations only:
Within this model, R _{ xy } and M _{ z } appear at T _{0R} and T _{0M}, respectively. On cooling, they progressively develop within the Pbnm phase and renormalize the energy curvature α _{B} of B _{OC} as made clear when grouping the \(Q_{\mathrm{B}}^2\) terms in Eq. (1):
When reaching a critical amplitude at which \(\tilde \alpha _{\mathrm{B}} = 0\), they trigger the appearance of B _{OC} and produce concurrent structural and metalinsulator phase transitions. The phase transition appears to be second order within this model, which is however too simple to be conclusive on this point (Supplementary Note 10).
All parameters and their evolution with R were directly fitted from first principles; only Curie temperatures were uniformly scaled to reproduce the experimental T _{MI} of YNiO_{3} (Supplementary Note 8). The phase diagram of nickelates as predicted within this model is reported in Fig. 3. This figure demonstrates that the cooperative coupling of B _{OC} with R _{ xy } and M _{ z } is a key mechanism that, by itself, accounts for the experimentally observed evolution of T _{MI} with the tolerance factor.
Hence, the MIT in nickelates turns out to be a concrete example of triggered phase transition^{26, 27}, a kind of transition never identified before in simple perovskites. Indeed, although biquadratic interactions are generic in this class of compounds, different distortions usually compete and exclude each other^{9}. The cooperative coupling of B _{OC} with oxygen rotations pointed out here is therefore an unusual and intriguing feature, whose origin is now traced back in the electronic band structure.
Electronic origin of the triggered mechanism
In the cubic phase, as expected from the formal Ni 3d ^{7} \(\left( {t_{{\mathrm{2g}}}^6e_{\mathrm{g}}^1} \right)\) occupancy, the Fermi energy E _{f} crosses levels of dominant Ni 3de _{g} character (i.e., antibonding Ni 3dO 2p states); such levels form an isolated and rather dispersive set of two e _{g} bands, shifted above the t _{2g} levels by the crystal field (Fig. 4). Forcing into this cubic structure a B _{OC} distortion, associated to a phonon at q _{R} = (1/2, 1/2, 1/2), can open a gap at q _{c} = (1/4, 1/4, 1/4) within the e _{g} bands but well above E _{f} and without any direct impact on the metallic character and the occupied states. Nevertheless, the oxygen rotation motions substantially affect the e _{g} bands (Fig. 4), reducing their bandwidth and yielding a progressive down shift of the e _{g} levels at q _{c}. As the rotations gradually increase and the bandwidth decreases, B _{OC} more substantially pushes down the electronic states around E _{f}, providing a progressive gain of electronic energy, which, in turn, results in the softening of ω _{B}. The critical rotation amplitude at which B _{OC} becomes unstable \(\left( {\tilde \alpha_{\mathrm{B}} = 0} \right)\) is precisely that at which the e _{g} levels at q _{c} cross E _{f}. At these amplitudes, the electronic system itself becomes unstable; the appearance of B _{OC} is favored and opens a gap at E _{f}, making the system insulating. As such, the MIT can therefore be interpreted as a Peierls instability but one that is not initially present and has been triggered by oxygen rotations.
Discussion
For compounds with small R cations, Q _{R} and Q _{M} are large and able to produce the MIT at relatively high temperatures, well above T _{N}. For large cations (R = Nd, Pr), oxygen rotations are reduced and, from our Landau model (built on FM results), no more sufficient to trigger the MIT (Fig. 3). However, as previously mentioned, the AFME′ spin order is compatible by symmetry with B _{OC} and induces its appearance as an improper order (linear shift of B _{OC} SW, Fig. 1d). Hence, although not opening a gap in the cubic phase, the onset of the AFME′ order in the Pbnm phase of NdNiO_{3} and PrNiO_{3} promotes the occurrence of the MIT almost triggered by the rotations. In these compounds, we have therefore T _{MI} = T _{N}; the transition is more abrupt and firstorder^{8}. Such active role of magnetism for large cations is supported by the experimental results and discussion in ref. ^{28}. It is also confirmed by our firstprinciples calculations on NdNiO_{3}, showing that the predicted T _{MI} is rescaled when including the change of magnetic order: while the system prefers to stay in the Pbnm metallic phase when imposing a FM order, it switches to the P2_{1}/n phase when adopting a AFME′ order. The cooperative effect of the magnetic order remains true for small cations but without any impact on T _{MI} (>T _{N}).
In conclusion, the concurrent electronic and structural transitions at T _{MI} in RNiO_{3} compounds take the form of a Peierls instability, which, primarily, is structurally triggered by the oxygen rotation motions R _{ xy } and M _{ z } and, eventually, is further assisted by the appearance of the E′type AFM magnetic ordering. Our Landau model, and its possible extension to incorporate explicitly strain degrees of freedom neglected here for simplicity, provides a simple and useful quantitative tool to estimate and interpret how T _{MI} can be tuned toward the monitoring of oxygen rotation motions R _{ xy } and M _{ z } when making solid solutions^{10}, applying pressure^{8}, or playing with the epitaxial strain and the orientation of the substrate in thin films^{29}. Our findings are relevant to other families of perovskites like A^{2+} Fe^{4+} O_{3} compounds^{30}. For instance, they can explain why CaFeO_{3}, which exhibits oxygen rotations, undergoes a MIT while SrFeO_{3} and BaFeO_{3}, which stay cubic, remain metallic. In addition, the same physics is also inherent to manganites like LaMnO_{3}, suggesting a close competition between charge and orbital orderings in this family compounds. However, the situation is slightly different in a bismutate like BaBiO_{3}, in which B _{OC} is intrinsically unstable in the cubic phase^{31}.
Methods
Firstprinciples calculations
Firstprinciples calculations were performed in the framework of DFT^{32, 33} using a Projected Augmented Wave (PAW) approach^{34} as implemented within the ABINIT package^{35,36,37,38}. The calculations relied on the Generalized Gradient Approximation using the PBEsol^{39} exchangecorrelation functional. We worked within a collinear spin approximation. We included a Hubbard correction U = 1.5 eV^{40} on the 3d orbitals of Ni atoms. A special care was devoted to the determination of the appropriate U parameter (Supplementary Notes 1– 4).
We made use of JTH atomic potentials^{41}. For the wavefunctions, we used an energy cutoff of 24 Ha (38 Ha for the second grid in the PAW spheres), which guarantees a convergence better than 1 meV on the total energy. The BZ was sampled with kpoint meshes equivalent to a 12 × 12 × 12 grid in the fiveatom unit cell. During structural relaxations, thresholds of 10^{−5} Ha/bohr on the maximum force and of 10^{−7} Ha/bohr^{3} on the maximum stress have been considered.
Structural analysis
The Goldschmidt tolerance factor^{42}, t = d _{R−O}/\(\sqrt 2\) d _{Ni−O}, of RNiO_{3} compounds were determined using Nicole Benedek’s tool^{43} relying on a bond valence model^{44} to calculate d _{R−O} and d _{Ni−O}, respectively, the ideal R–O and Ni–O bond lengths in the cubic perovskite structure.
Symmetryadapted mode analysis have been performed with AMPLIMODE^{45, 46}. The modes are normalized to their amplitude in the P2_{1}/n AFME′ ground state. This normalization is such that in cubic phase (volume of the ground state) Q _{R} = 100% corresponds to rotation angles ϕ _{ x } = ϕ _{ y } = 11.33° (Ni–O–Ni angle of 157.33°), Q _{R} = 100% corresponds to a rotation angle ϕ _{ z } = 12.12° (Ni–O–Ni angle of 155.75°) and Q _{B} = 100% corresponds to oxygen displacements d _{O} = 0.0358.
Landau model
The Landau model parameters have been fitted for YNiO_{3}, GdNiO_{3}, and SmNiO_{3} on firstprinciples data using in each case a FM cubic phase (volume of the ground state) and interpolated for the other compounds. T _{MI} was determined analytically (Supplementary Notes 6–9).
Data availability
All relevant data are available from the authors.
References
Demazeau, G., Marbeuf, A., Pouchard, M. & Hagenmuller, P. Sur une série de composés oxygènes du nickel trivalent derivés de la perovskite. J. Solid State Chem. 3, 582 (1971).
Shi, J., Ha, S. D., Zhou, Y., Schoofs, F. & Ramanathan, S. A correlated nickelate synaptic transistor. Nat. Commun. 4, 2676 (2013).
Zhou, Y. et al. Strongly correlated perovskite fuel cells. Nature 534, 231–234 (2016).
Middey, S. et al. Physics of ultrathin films and heterostructures of rareearth nickelates. Annu. Rev. Mater. Res. 46, 305–334 (2016).
Först, M. et al. Spatially resolved ultrafast magnetic dynamics initiated at a complex oxide heterointerface. Nat. Mater. 14, 883–888 (2015).
Kim, T. H. et al. Polar metals by geometric design. Nature 533, 68–72 (2016).
Grisolia, M. N. et al. Hybridizationcontrolled charge transfer and induced magnetism at correlated oxide interfaces. Nat. Phys. 12, 484–492 (2016).
Catalan, G. Progress in perovskite nickelate research. Phase Transit. 81, 729–749 (2008).
Benedek, N. A. & Fennie, C. J. Why are there so few perovskite ferroelectrics? J. Phys. Chem. C 117, 13339–13349 (2013).
Medarde, M. L. Structural, magnetic and electronic properties of RniO_{3} perovskites (R = rare earth). J. Phys. Condens. Matter 9, 1679 (1997).
Alonso, J. A. et al. Charge disproportionation in RniO _{ 3 } perovskites: simultaneous metalinsulator and structural transition in YNiO _{ 3 }. Phys. Rev. Lett. 82, 3871–3874 (1999).
GarcíaMuñoz, J. L., RodríguezCarvajal, J. & Lacorre, P. Neutrondiffraction study of the magnetic ordering in the insulating regime of the perovskites RniO_{3} R = Pr and Nd). Phys. Rev. B 50, 978–992 (1994).
Lee, S., Chen, R. & Balents, L. Landau theory of charge and spin ordering in the nickelates. Phys. Rev. Lett. 106, 016405 (2011).
Torrance, J. B., Lacorre, P., Nazzal, A. I., Ansaldo, E. J. & Niedermayer, C. Systematic study of insulatormetal transitions in perovskites RniO_{3} R = Pr, Nd, Sm, Eu) due to closing of chargetransfer gap. Phys. Rev. B 45, 8209–8212 (1992).
Mizokawa, T., Khomskii, D. I. & Sawatzky, G. A. Spin and charge ordering in selfdoped Mott insulators. Phys. Rev. B 61, 11263–11266 (2000).
Raebiger, H., Lany, S. & Zunger, A. Charge selfregulation upon changing the oxidation state of transition metals in insulators. Nature 453, 763–766 (2008).
Park, H., Millis, A. J. & Marianetti, C. A. Siteselective mott transition in rareearthelement nickelates. Phys. Rev. Lett. 109, 156402 (2012).
Ruppen, J. et al. Optical spectroscopy and the nature of the insulating state of rareearth nickelates. Phys. Rev. B 92, 155145 (2015).
Varignon, J., Grisolia, M. N., Iniguez, J., Barthélémy, A. & Bibes, M. Complete phase diagram of rareearth nickelates from first principles. npj Quant. Mater. 2, 21 (2017).
Mazin, I. I. et al. Charge ordering as alternative to jahnteller distortion. Phys. Rev. Lett. 98, 176406 (2007).
Johnston, S., Mukherjee, A., Elfimov, I., Berciu, M. & Sawatzky, G. A. Charge disproportionation without charge transfer in the rareearthelement nickelates as a possible mechanism for the metalinsulator transition. Phys. Rev. Lett. 112, 106404 (2014).
Bisogni, V. et al. Ground state oxygen holes and the metalinsulator transition in the negative charge transfer rareearth nickelates. Nat. Commun. 7, 13017 (2016).
de la Cruz, F. P. et al. Possible common ground for the metalinsulator phase transition in the rareearth nickelates RniO_{3} (R = Eu, Ho, Y). Phys. Rev. B 66, 153104 (2002).
Balachandran, P. V. & Rondinelli, J. M. Interplay of octahedral rotations and breathing distortions in chargeordering perovskite oxides. Phys. Rev. B 88, 054101 (2013).
Holakovsky, J. A new type of ferroelectric phase transition. Phys. Status Solidi B 56, 615–619 (1973).
Flerov, I. N., Gorev, M. V., Voronov, V. N., Tressaud, A. & Grannec, J. Triggered phase transitions in Rb_{2}KB^{3+}F_{6}(B^{3+}: Er, ho) elpasolites. J. Solid State Chem. 3, 582 (1971).
Iwata, M., Zhao, C. H., Aoyagi, R., Maeda, M. & Ishibashi, Y. Splitting of triggered phase transition in Bi_{4−x }La_{ x }Ti_{3}O_{12} mixed crystals. Japonese. J. Appl. Phys. 46, 5894 (2007).
Vobornik, I. et al. Electronicstructure evolution through the metalinsulator transition in RniO_{3}. Phys. Rev. B 60, R8426–R8429 (1999).
Catalano, S. et al. Tailoring the electronic transitions of NdNiO_{3} films through (111)pc oriented interfaces. APL Mater. 3, 062506 (2015).
Akao, T. et al. Chargeordered state in singlecrystalline CaFeO_{3} thin film studied by xray anomalous diffraction. Phys. Rev. Lett. 91, 156405 (2003).
Liechtenstein, A. I. et al. Structural phase diagram and electronphonon interaction in Ba_{1−x }K_{ x }BiO_{3}. Phys. Rev. B 44, 5388–5391 (1991).
Hohenberg, P. & Kohn, W. Inhomogeneous electron gas. Phys. Rev. 136, B864–B871 (1964).
Kohn, W. & Sham, L. J. Selfconsistent equations including exchange and correlation effects. Phys. Rev. 140, A1133–A1138 (1965).
Blöchl, P. E. Projector augmentedwave method. Phys. Rev. B 50, 17953–17979 (1994).
Gonze, X. et al. ABINIT: Firstprinciples approach to material and nanosystem properties. Comput. Phys. Commun. 180, 2582–2615 (2009).
Gonze, X. et al. Firstprinciples computation of material properties: the ABINIT software project. Computat. Mater. Sci. 25, 478–492 (2002).
Gonze, X. et al. A brief introduction to the abinit software package. Z. Kristallogr. Cryst. Mater. 220, 558–562 (2005).
Torrent, M., Jollet, F., Bottin, F., Zérah, G. & Gonze, X. Implementation of the projector augmentedwave method in the ABINIT code: application to the study of iron under pressure. Comput. Mater. Sci. 42, 337–351 (2008).
Perdew, J. P. et al. Restoring the densitygradient expansion for exchange in solids and surfaces. Phys. Rev. Lett. 100, 136406 (2008).
Liechtenstein, A. I., Anisimov, V. I. & Zaanen, J. Densityfunctional theory and strong interactions: orbital ordering in motthubbard insulators. Phys. Rev. B 52, R5467–R5470 (1995).
Jollet, F., Torrent, M. & Holzwarth, N. Generation of Projector AugmentedWave atomic data: a 71 element validated table in the XML format. Comput. Phys. Commun. 185, 1246–1254 (2014).
Goldschmidt, V. M. Die gesetze der krystallochemie. Naturwissenschaften 14, 477–485 (1926).
Benedek, N. Tolerance factor calculator v0.2.1.
Lufaso, M. W. & Woodward, P. M. Prediction of the crystal structures of perovskites using the software program spuds. Acta. Crystallogr. B. 57, 725 (2001).
Orobengoa, D., Capillas, C., Aroyo, M. I. & PerezMato, J. M. AMPLIMODES: symmetrymode analysis on the Bilbao Crystallographic Server. J. Appl. Crystallogr. 42, 820–833 (2009).
PerezMato, J. M., Orobengoa, D. & Aroyo, M. I. Mode crystallography of distorted structures. Acta Crystallogr. A 66, 558–590 (2010).
Acknowledgements
We thank Y. Zhang, E. Bousquet, F. Ricci, M. Verstraete, J.Y. Raty, S. Catalano, J.M. Triscone, A. Georges and J. Varignon for fruitful discussions. This work was supported by FRSFNRS project HiT4FiT and ARC project AIMED. J.I. acknowledges support form FNR Luxembourg Grant P12/4853155 “COFERMAT”. Calculations have been performed on the Céci facilities funded by F.R.SFNRS (Grant No 2.5020.1) and Tier1 supercomputer of the Fédération WallonieBruxelles funded by the Walloon Region (Grant No 1117545). They also took advantage of HPC resources from the French Research and Technology Computing Center (CCRT) and from the PRACE project Megapasta.
Author information
Authors and Affiliations
Contributions
P.G. conceived the study with A.M. and J.I. and directed the work. A.M. and J.B. did the firstprinciples simulations. A.M. and P.G. did the Landau modeling. P.G. wrote the manuscript with A.M. and J.B. All authors discussed the results at different stages of the study and commented on the manuscript.
Corresponding author
Ethics declarations
Competing interests
The authors declare no competing financial interests.
Additional information
Publisher's note: Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Electronic supplementary material
Rights and permissions
Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/.
About this article
Cite this article
Mercy, A., Bieder, J., Íñiguez, J. et al. Structurally triggered metalinsulator transition in rareearth nickelates. Nat Commun 8, 1677 (2017). https://doi.org/10.1038/s4146701701811x
Received:
Accepted:
Published:
DOI: https://doi.org/10.1038/s4146701701811x
This article is cited by

Quantifying the role of the lattice in metal–insulator phase transitions
Communications Physics (2022)

Persistent halfmetallic ferromagnetism in a (111)oriented manganite superlattice
npj Computational Materials (2022)

Hole doping in a negative charge transfer insulator
Communications Physics (2022)

Nonuniversal current flow near the metalinsulator transition in an oxide interface
Nature Communications (2021)

Annealing temperatures effect on the electrical and structural properties of nanocrystalline vanadium dioxide films prepared by Sol–Gel technique
Applied Physics A (2021)
Comments
By submitting a comment you agree to abide by our Terms and Community Guidelines. If you find something abusive or that does not comply with our terms or guidelines please flag it as inappropriate.